Resistance welding of aluminium by abd al rahman ata
Suitability of Aluminium and its alloys for spot welding
• The suitability of aluminium and its alloys for spot welding depends mainly on 3
- surface conditions
- chemical composition
- metallurgical conditions
• Because of its high affinity to oxygen, the free surface of aluminium is covered by a
dense, tightly adhering oxide film.
• This film is a non-conductor of electricity and must, therefore, be removed prior to
• This is generally accomplished mechanically by brushing or chemically by etching.
• The oxide film, if it comes in direct contact with the contacting electrode, would lead
to a local accumulation of heat at the contacting region and metal pick-up on
electrode, i.e., the electrode life would be very limited.
Both electrical and thermal conductivity depend strongly on the
chemical composition. The very good electrical conductivity of pure
aluminium makes it necessary to use large currents. Consequently,
both thermal stressing and electrode wear are high. The state of a
metal, whether hard or soft, depends on its metallurgical condition.
Cold worked aluminium can generally be better spot-welded than
aluminium in a soft condition
Due to the high thermal conductivity of aluminium, a large portion
of the heat created is absorbed by the cooled electrode and the
surrounding material. Consequently, a stationary state of equilibrium
between the heat input and output is reached within a short welding
time. For this reason, it is essential that the welding energy for
aluminium be delivered within as short a time as possible. Thus, the
current required for welding aluminium is about twice that for
welding steel sheets of the same thickness, and this although the
aluminium alloys have a much lower melting point.
Resistances during Spot Welding of Steel and Aluminium
The formation of the weld nugget depends mainly on the current strength, the resistance and
the welding time. The heat generated can be calculated using Joule's law:
Q = 0.23 × I² × R × t
The total resistance is made up of the contact resistances and the material resistances. The
material resistances of the sheets and the contact resistances between the sheets themselves and
between sheet and electrode have very different orders of magnitude for aluminium and steel.
The welding parameters (current, time, force) have thus to be adapted for the higher electrical
and thermal conductivities of aluminium.
An intensive cooling of the electrodes is of paramount importance to avoid any
electrode metal pick-up tendency.
Due to the low resistance of the material aluminium, the spot welding must be carried out with
high welding currents within short welding times using a special electrode force program
Constitution of the Oxide Film
The high affinity of aluminium for oxygen, which causes metallic blank aluminium
to be covered at once with a thin, dense and tightly adhering oxide film, has a major
effect on the suitability of aluminium for spot welding.
The oxide film has a high thermal stability and a melting temperature of over
2,000°C and is a non-conductor of electricity. Diffusion processes govern the
formation and growth of this oxide film; its thickness increases in proportion to the
square-root of time.
The oxide film consists of an almost pore-free barrier layer and a covering porous
oxide layer. The typical thicknesses lie between 0.005 and 0.01 µm
During welding, the high electrode contact
pressure causes the sheet surfaces to be
deformed locally. This causes the brittle
oxide film to crack, so that the welding
current can now flow through the fine
contact bridges; due to the heat developed
and the continuing deformation, the
contact bridges are enlarged, causing the
contact resistance to fall rapidly.
Cleaning Drying Etching Rinsing Passivation
Most of the etchants used also attack the metallic aluminium once the oxide skin is
removed and, if the contact time is long enough, form a new coating layer which once
again increases the contact resistance. Therefore, the etching parameters must be
strictly adhered to and followed by a thorough rinsing by spraying with cold or
warm (preferably deionised) water.
Contact Resistance after Surface Pretreatment
A proper surface pretreatment can reduce the contact resistance between electrode
and sheet to values between 3 and 50 µΩ
Alkaline solutions, with10 to 20 %
sodium hydroxide solution and mixed
acids, are the most commonly used
Resulting in the optimum etching time
to be less critical
During direct current welding, the Peltier effect occurs, causing a larger electrode wear at the anode
than at the cathode. This effect is caused by the heat consumed during transfer of electricity at the
contact cathode-sheet and the heat released at the contact anode-sheet. This difference in reactions is
caused by the corresponding positions of aluminium and copper in the electrochemical potential series.
The additional heat released at the anode leads to a higher thermal stressing and to lower electrode life
In order to minimize this effect, welding
machines have been developed in which the
electrode polarity is changed after each spot
Current-Force Diagram for Spot Welding Aluminium
A current-force program in which both parameters change with time, is used to produce welds of high
An initial force is applied to ensure a good contact between sheet and electrode, thereby reducing the
contact resistance. The force is then lowered, i.e., the contact resistance between the sheets increases,
and the current is allowed to flow.
The rate of current increase (up slope), amplitude, time and current decrease rate (down slope) can be
regulated to suit the alloy to be welded
Heating of the metals during current flow causes these to soften, so that the force decreases. Shortly
after the maximum current is reached, the force is increased to press the sheets against each other
(forging effect). Similar programs are mandatory for welding in the aerospace industry
The currents used for aluminium are much higher than those required for spot
welding steel, making it necessary to utilize machines with a higher power
rating for spot welding aluminium.
The type of material used for the electrodes has a significant influence
on the operational life. Experience has proved that material strength and
hardness are of greater importance than the electrical conductivity.
Recommended Values for Spot Welding with Direct Current
Because of the high thermal conductivity of aluminium, the welding times chosen should be as short
as possible to prevent the formation of a stationary state of equilibrium in which the input heat is
absorbed by the material and is thus no longer available for the formation of the weld nugget.
This means that very high welding currents have to be used.
Since aluminium has a lower hardness than steel, the electrode forces required for spot welding are
lower. High forces would cause unallowable electrode indentations in the aluminium.
Effect of Weld Spot Diameter on the Shear Strength
The load-carrying capacity of the joint depends on the weld spot diameter.
Depending on the welded materials, weld spot diameter and shear strength increase
Heat-treatable alloys which have been age hardened, lose this hardening effect in the
heat affected zone of the weld.
A heat treatment of such components is, in principle, possible but its practical use is
strongly limited by the part size and possible distortion expected.
Therefore, the unavoidable loss in strength is
compensated for by increasing the weld spot diameter.
Larger weld spot diameters are necessary to attain the
required shear strength with softer materials
Correlations between Surface Pretreatment, Weld Strength
The mechanical pretreatment can be carried out with simple equipment and does not require any
The softer alloys (pure aluminium, AlMn) tend to "smear" easily so that proper care must be taken
while working with them.
The same care must be taken for plated alloys, in order to prevent a mechanical removal of the thin
Small areas can be mechanically pretreated with hand-held or rotating (ø > 200 mm) brushes made of
stainless steel or also with steel wool.
Grinding is carried out using grinding wheels or grinding bands. Abrasive powder with uniform
particle size is used to obtain a fine surface finish.
Overheating is prevented by using moderate grinding pressures, appropriate operating speeds (30 to
40 m/min) as well as by introducing additives (fat, paraffin) to the abrasive powder.
A disadvantage of mechanical surface pretreatments is the roughening of
The contact resistance can only be reduced down to 50 to 100 µΩ, the
associated heating at the interface electrode/sheet surface leads to electrode
The mechanical pretreatment produces an active surface which oxidizes
rapidly to form a new oxide film.
Consequently, the contact resistance rises sharply within short storage
times, increases of 20 µΩ occurring within about 20 min
Repeated Tensile Stress Fatigue Strength of One-Spot Samples
The fatigue behaviour of materials can be ascertained at values of 2 x 107
cycles and more.
Weld defects like pores and cavities which are not located at the weld nugget
edges have hardly any influence.
Cracks and reductions in cross-section due to too high electrode pressures,
reduce the fatigue strength sharply.
The amount of overlap also has a significant effect on the
Fatigue Strength of Spot Welded 1.6 mm Thick 2024 cl Sheets
Experiments have shown that the effect of specimen form on the fatigue strength is much greater
than that of other variables like lower or higher current, cracks, corrosion etc.
The effect of the added bending due to specimen form is clearly visible. Therefore, a careful
evaluation of the results is essential
Allowable Imperfections of Spot Welds in Aluminium
Alloys Determined by Metallography
• The geometrical characteristics and
allowable defect dimensions for spot welds
depend on the corresponding evaluation
group (EG). The EG I has the strictest
requirements (crack and inclusions are not
allowed in this evaluation group)
Allowable Imperfections of Spot Welds in Aluminium Alloys
Determined by X-Ray Examination
Inclusions and cavities can also be determined using the radiographic testing
method. An important factor here is the location distance of the defect from the
Defects located within the interior of the weld spot have a lower notch effect and
are therefore not as dangerous as those located at the spot boundaries
Bad shape of welding
Deep indentation of welding
electrodes in sheets